K<sub>2</sub>TeP<sub>2</sub>O<sub>8</sub>: a new telluro-phosphate with a pentagonal Te-P-O layer structure.
Wen, Ming; Hu, Cong; Yang, Zhihua; Wu, Xiaohong; Pan, Shilie; Dalton transactions (Cambridge, England : 2003) 47 (2018) 9453–9458; doi:10.1039/c8dt01576g

data_7046714
_publ_section_title
;
 K<sub>2</sub>TeP<sub>2</sub>O<sub>8</sub>: a new telluro-phosphate with a
 pentagonal Te-P-O layer structure.
;
_journal_issue                   28
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9453
_journal_page_last               9458
_journal_paper_doi               10.1039/c8dt01576g
_journal_volume                  47
_journal_year                    2018
_chemical_absolute_configuration rm
_chemical_formula_sum            'K2 O8 P2 Te'
_chemical_formula_weight         395.74
_space_group_crystal_system      orthorhombic
_space_group_IT_number           18
_space_group_name_Hall           'P 2 2ab'
_space_group_name_H-M_alt        'P 21 21 2'
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.9684(5)
_cell_length_b                   12.1871(5)
_cell_length_c                   5.5283(2)
_cell_measurement_reflns_used    3456
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.45
_cell_measurement_theta_min      3.34
_cell_volume                     806.36(6)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0216
_diffrn_reflns_av_unetI/netI     0.0270
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            4961
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.473
_diffrn_reflns_theta_min         2.385
_exptl_absorpt_coefficient_mu    5.129
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.6574
_exptl_absorpt_correction_type   numerical
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.260
_exptl_crystal_description       block
_exptl_crystal_F_000             736
_exptl_crystal_size_max          0.114
_exptl_crystal_size_mid          0.095
_exptl_crystal_size_min          0.093
_refine_diff_density_max         1.341
_refine_diff_density_min         -1.584
_refine_diff_density_rms         0.166
_refine_ls_abs_structure_details
; 
 Refined as an inversion twin. 
;
_refine_ls_abs_structure_Flack   0.01(6)
_refine_ls_extinction_coef       0.0060(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   0.983
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     125
_refine_ls_number_reflns         1843
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.017
_refine_ls_R_factor_all          0.0315
_refine_ls_R_factor_gt           0.0306
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+10.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0701
_refine_ls_wR_factor_ref         0.0707
_reflns_Friedel_coverage         0.678
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                1793
_reflns_number_total             1843
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8dt01576g1.cif
_cod_data_source_block           1
_cod_depositor_comments          'Adding full bibliography for 7046714.cif.'
_cod_database_code               7046714
_shelx_shelxl_version_number     2016/6
_shelx_res_checksum              55031
_shelx_hkl_checksum              62883